DOI: 10.17188/1475748
title: Materials Data on Sr2Ca6TiMn7O20 by Materials Project

description: Sr2Ca6TiMn7O20 crystallizes in the triclinic P1 space group. The structure is three-dimensional. there are eight inequivalent Sr2+ sites. In the first Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.44–3.12 Å. In the second Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.44–3.16 Å. In the third Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.40–2.81 Å. In the fourth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.42–3.11 Å. In the fifth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.48–3.00 Å. In the sixth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.44–3.16 Å. In the seventh Sr2+ site, Sr2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Sr–O bond distances ranging from 2.41–2.87 Å. In the eighth Sr2+ site, Sr2+ is bonded in a 9-coordinate geometry to nine O2- atoms. There are a spread of Sr–O bond distances ranging from 2.46–3.13 Å. There are twenty-four inequivalent Ca2+ sites. In the first Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.31–2.94 Å. In the second Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.30–2.82 Å. In the third Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.31–2.91 Å. In the fourth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.27–3.01 Å. In the fifth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.31–2.93 Å. In the sixth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.80 Å. In the seventh Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.83 Å. In the eighth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.84 Å. In the ninth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.27–3.02 Å. In the tenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.34–2.86 Å. In the eleventh Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.24–2.94 Å. In the twelfth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.33–2.89 Å. In the thirteenth Ca2+ site, Ca2+ is bonded in a 5-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.31–2.91 Å. In the fourteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.29–2.92 Å. In the fifteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.29–2.90 Å. In the sixteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.29–2.99 Å. In the seventeenth Ca2+ site, Ca2+ is bonded in a 2-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.30–2.97 Å. In the eighteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.79 Å. In the nineteenth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.82 Å. In the twentieth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.37–2.87 Å. In the twenty-first Ca2+ site, Ca2+ is bonded in a 7-coordinate geometry to seven O2- atoms. There are a spread of Ca–O bond distances ranging from 2.25–2.80 Å. In the twenty-second Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.26–2.85 Å. In the twenty-third Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.36–2.92 Å. In the twenty-fourth Ca2+ site, Ca2+ is bonded in a 8-coordinate geometry to eight O2- atoms. There are a spread of Ca–O bond distances ranging from 2.30–2.86 Å. There are four inequivalent Ti4+ sites. In the first Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share a cornercorner with one TiO6 octahedra, corners with three MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 12–18°. There are a spread of Ti–O bond distances ranging from 1.94–2.00 Å. In the second Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share a cornercorner with one TiO6 octahedra, corners with three MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–15°. There are a spread of Ti–O bond distances ranging from 1.95–2.00 Å. In the third Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share a cornercorner with one TiO6 octahedra, corners with three MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–17°. There are a spread of Ti–O bond distances ranging from 1.94–2.02 Å. In the fourth Ti4+ site, Ti4+ is bonded to six O2- atoms to form TiO6 octahedra that share a cornercorner with one MnO6 octahedra, corners with three TiO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–18°. There are a spread of Ti–O bond distances ranging from 1.89–2.11 Å. There are twenty-eight inequivalent Mn+2.86+ sites. In the first Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 6–10°. There are a spread of Mn–O bond distances ranging from 1.94–2.11 Å. In the second Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–11°. There are a spread of Mn–O bond distances ranging from 1.95–2.07 Å. In the third Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 9–13°. There are a spread of Mn–O bond distances ranging from 1.94–2.05 Å. In the fourth Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one TiO6 octahedra, corners with three MnO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one MnO4 trigonal pyramid. The corner-sharing octahedra tilt angles range from 8–13°. There are a spread of Mn–O bond distances ranging from 2.00–2.05 Å. In the fifth Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 7–12°. There are a spread of Mn–O bond distances ranging from 1.94–2.05 Å. In the sixth Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one MnO6 octahedra, corners with three TiO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–15°. There are a spread of Mn–O bond distances ranging from 1.94–2.19 Å. In the seventh Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one MnO4 trigonal pyramid. The corner-sharing octahedra tilt angles range from 6–11°. There are a spread of Mn–O bond distances ranging from 1.96–2.05 Å. In the eighth Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one MnO6 octahedra, corners with three TiO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 8–12°. There are a spread of Mn–O bond distances ranging from 1.90–2.23 Å. In the ninth Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 8–13°. There are a spread of Mn–O bond distances ranging from 1.96–2.01 Å. In the tenth Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share a cornercorner with one MnO6 octahedra, corners with three TiO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 10–12°. There are a spread of Mn–O bond distances ranging from 1.90–2.22 Å. In the eleventh Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 8–12°. There are a spread of Mn–O bond distances ranging from 1.98–2.02 Å. In the twelfth Mn+2.86+ site, Mn+2.86+ is bonded to six O2- atoms to form MnO6 octahedra that share corners with four MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 6–12°. There are a spread of Mn–O bond distances ranging from 1.95–2.03 Å. In the thirteenth Mn+2.86+ site, Mn+2.86+ is bonded to four O2- atoms to form MnO4 tetrahedra that share a cornercorner with one TiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 30–36°. There are a spread of Mn–O bond distances ranging from 2.00–2.08 Å. In the fourteenth Mn+2.86+ site, Mn+2.86+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two MnO6 octahedra and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 21–30°. There are a spread of Mn–O bond distances ranging from 1.86–1.98 Å. In the fifteenth Mn+2.86+ site, Mn+2.86+ is bonded to four O2- atoms to form MnO4 tetrahedra that share a cornercorner with one TiO6 octahedra, a cornercorner with one MnO6 octahedra, and corners with two MnO4 tetrahedra. The corner-sharing octahedra tilt angles range from 31–32°. There are a spread of Mn–O bond distances ranging from 2.00–2.10 Å. In the sixteenth Mn+2.86+ site, Mn+2.86+ is bonded to four O2- atoms to form MnO4 tetrahedra that share corners with two MnO6 octahedra, a cornercorner with one MnO4 tetrahedra, and a cornercorner with one MnO4 trigonal pyramid. The corner-sharing octahedra tilt angles range from 22–30°. There are a spread of Mn–O bond distances ranging from 1.89–1.99 Å. In the seventeenth Mn+2.86+ site, Mn+2.86+ is bonded to four O2- atoms to form MnO4 tetrahedra that share a cornercorner with one TiO6 octahedra, a cornercorner with one M